**Table 1.**

temperature showing an intense blue fluorescence with high fluorescent quantum yield, independent of the excitation wavelength in different solvents. The spectra clearly reveal that the emission originate from an excited state-charge transfer state π-π\* because of the presence of N atoms. Thus, the compound phh may be a

*Strongly Fluorescent Heterocyclic Molecule: Crystallography, 3D Hydrogen-Bonded, Fluorescence…*

All geometry optimizations of the molecular structure of phh were performed within the Amsterdam Density Functional (ADF) software [9], and all of theoretical calculations were carried out by the density functional theory (DFT), using the Perdew, Burke and Ernzerhof's exchange functional along with generalized gradient

Singlet excited states were optimized using time-dependent DFT (TD-DFT)

The geometric optimization has been carried on the molecular structure of phh. The ground state geometry was adapted from the X-ray data. Calculated structural parameters reveal a good agreement with the original X-ray diffraction data, which

The time-dependent density functional theory calculations were performed on this compound, with the aim to identify the nature of the electronic transitions.

N1A▬C1A 1.32 (4) N2B▬C10B 1.34 (5) N1A▬C12A 1.36 (4) N2B▬C11B 1.36 (4) N2A▬C10A 1.32 (4) N1C▬C12C 1.35 (4) N2A▬C11A 1.36 (4) N1C▬C1C 1.33 (4) N1B▬C12B 1.36 (4) N2C▬C11C 1.36 (4) N1B▬C1B 1.32 (5) N2C▬C10C 1.33 (4) C1A▬N1A▬C12A 117 (3) N1B▬C1B▬C2B 124 (3) C10A▬N2A▬C11A 117 (3) N2B▬C10B▬C9B 123 (3) C1B▬N1B▬C12B 119 (3) N2B▬C11B▬C7B 123 (3) C10B▬N2B▬C11B 117 (3) N2B▬C11B▬C12B 118 (2) C1C▬N1C▬C12C 117 (2) N1B▬C12B▬C11B 119 (3) C10C▬N2C▬C11C 117 (3) N1B▬C12B▬C4B 122 (3) N1A▬C1A▬C2A 124 (3) N1C▬C1C▬C2C 124 (3) N2A▬C10A▬C9A 125 (4) N2C▬C10C▬C9C 125 (3) N2A▬C11A▬C7A 123 (3) N2C▬C11C▬C7C 123 (3) N2A▬C11A▬C12A 118 (3) N2C▬C11C▬C12C 118 (2) N1A▬C12A▬C4A 123 (3) N1C▬C12C▬C4C 124 (3) N1A▬C12A▬C11A 118 (3) N1C▬C12C▬C11C 118 (2)

approximations, exchange and correlation functional GGA (PBE) [10, 11],

candidate for blue-light luminescent materials.

*DOI: http://dx.doi.org/10.5772/intechopen.90271*

employing the triple-zeta polarized (TZP) basis set.

indicates significant stability of both compounds (**Table 2**).

**5. Theoretical analysis**

calculations [12–15].

**Table 2.**

**81**

*Selected geometric parameters (Å,°).*

**5.1 TD-DFT absorption spectra**

#### **Figure 2.**

*(a) Partial view of the packing in the phh, showing the O▬H O, O▬H N, C▬H O and C▬H N hydrogen bonds. (b) Partial view of the packing in the phh, showing the formation of the infinite chain C3 3(7). (c) Graph set R<sup>2</sup> 1(5), R<sup>2</sup> 2(9), R<sup>5</sup> 6(22) and R<sup>4</sup> 6(15) motifs. Atoms are represented as circles of different radii. Hydrogen bonds are shown as dashed lines.*

#### **Figure 3.**

*Fluorescence spectra of phh in polar and non-polar solvent.*

440 nm, which resembles with the emission spectrum in non-polar solvents. This also indicates the absence of any aggregates or other conformers in the ground state. The studied compound was found to be fluorescently active in solution at room

*Strongly Fluorescent Heterocyclic Molecule: Crystallography, 3D Hydrogen-Bonded, Fluorescence… DOI: http://dx.doi.org/10.5772/intechopen.90271*

temperature showing an intense blue fluorescence with high fluorescent quantum yield, independent of the excitation wavelength in different solvents. The spectra clearly reveal that the emission originate from an excited state-charge transfer state π-π\* because of the presence of N atoms. Thus, the compound phh may be a candidate for blue-light luminescent materials.

## **5. Theoretical analysis**

All geometry optimizations of the molecular structure of phh were performed within the Amsterdam Density Functional (ADF) software [9], and all of theoretical calculations were carried out by the density functional theory (DFT), using the Perdew, Burke and Ernzerhof's exchange functional along with generalized gradient approximations, exchange and correlation functional GGA (PBE) [10, 11], employing the triple-zeta polarized (TZP) basis set.

Singlet excited states were optimized using time-dependent DFT (TD-DFT) calculations [12–15].

The geometric optimization has been carried on the molecular structure of phh. The ground state geometry was adapted from the X-ray data. Calculated structural parameters reveal a good agreement with the original X-ray diffraction data, which indicates significant stability of both compounds (**Table 2**).

#### **5.1 TD-DFT absorption spectra**


The time-dependent density functional theory calculations were performed on this compound, with the aim to identify the nature of the electronic transitions.

#### **Table 2.**

*Selected geometric parameters (Å,°).*

440 nm, which resembles with the emission spectrum in non-polar solvents. This also indicates the absence of any aggregates or other conformers in the ground state. The studied compound was found to be fluorescently active in solution at room

*(a) Partial view of the packing in the phh, showing the O▬H O, O▬H N, C▬H O and C▬H N hydrogen bonds. (b) Partial view of the packing in the phh, showing the formation of the infinite chain C3*

*6(15) motifs. Atoms are represented as circles of different radii.*

*3(7). (c)*

**Figure 2.**

*Graph set R<sup>2</sup>*

**Figure 3.**

**80**

*1(5), R<sup>2</sup>*

*Electron Crystallography*

*Hydrogen bonds are shown as dashed lines.*

*2(9), R<sup>5</sup>*

*Fluorescence spectra of phh in polar and non-polar solvent.*

*6(22) and R<sup>4</sup>*

The absorption spectra of the studied compound are shown in **Figure 1**. The computed absorption bands, dominant transitions, characters and oscillator strengths (f) are given in **Table 3**.

The compound phh that absorbs in the region (λ = 165–280 nm) appears in **Figure 4**, and it shows three peaks with maxima at λ = 190, 225 and 268. **Table 3** clearly indicates that the lowest energy and the intense peak is at λ = 268 nm (E = 4.62 eV), transition character as corresponding it results from a transition H2 to L+1**.** From **Figure 4** we observe two absorption peaks positioned at λ = 225 and 190 nm; the absorption bands correspond to the H1 to L+3 and H3 to L+2, respectively; and these transitions are affected to a π-π\* transition.

### **5.2 AIM topological analysis**

Bader and Essen have shown that that the negative value of ∇<sup>2</sup> (ρ) indicates that there is an electronic charge concentration at the BCP, which implies that the nature of the bond is covalent. For intermolecular interactions, is less weak and ∇ > 0, which implies the presence of a hydrogen-bonding interaction [16, 17].

The atoms in molecules (AIM) theory for part B (C1B to C12B/O1W) was applied to analyze the electron densities and their properties; details obtained from this approach are shown in **Table 4**. **Figure 5** shows the existence of a bond critical point between all of each two bonded atoms in part B.

We notice from **Table 4**, the values ρ > 0.2 and Δ < 0 indicate that covalent bonds are present. And for the bond between N1B and H11W, we notice that ρ = 0.034 is very weak and Δ = 0.091 > 0 (see **Table 4**) which indicate the presence of a strong hydrogen-bonding interaction. These results are in good agreement with those obtained by experimental refinement.


**5.3 Orbital analysis and molecular electrostatic potential**

*Results of atoms in molecule approach for part B of phh molecule.*

*DOI: http://dx.doi.org/10.5772/intechopen.90271*

B of compound phh is shown in **Figure 6**.

tions [18–21].

**83**

**Figure 5.**

**Table 4.**

(2.92 eV; see **Figure 6**) and predicts its stability.

*The critical point founded between every pair of atoms in part B.*

The energy diagram of the molecular orbitals obtained by DFT approach for part

The HOMO and LUMO are important orbitals in a molecule; the gap between the occupied and vacant orbitals (HOMO/LUMO) is remarkable in the compound

**Basins ρ ∇ |V|/G H** N1B▬H11W 0.034 0.091 1.063 0.001 N1B▬C1B 0.329 0.869 3.275 0.387 N1B▬C12B 0.341 0.946 3.138 0.444 O1W▬H1W 0.346 1.686 6.984 0.506 O1W▬H11W 0.327 1.685 7.426 0.499

*Strongly Fluorescent Heterocyclic Molecule: Crystallography, 3D Hydrogen-Bonded, Fluorescence…*

The highest occupied molecular orbital (HOMO) is mainly delocalized on the oxygen atom (93%), while it is found that the carbons of the cycles contribute strongly in the composition of the LUMO orbital with a participation rate of 88%. The molecular electrostatic potential is a very important element for the illustration and visualization of the charge region variability and allows identifying the electrophilic and nucleophilic attack sites as well as the hydrogen-bonding interac-

The blue region represents positive MESP, and the red region represents negative ESP, while the green region refers to the neutral region. From the MESP surface diagram, it can be seen that negative regions (red) are mainly localized over the oxygen and the nitrogen atom, while the positive regions (blue) are distributed over

**Table 3.**

*The calculated optical transition energies and their corresponding oscillator strengths (f) for phh.*

**Figure 4.** *TD-DFT absorption spectra of phh.*


*Strongly Fluorescent Heterocyclic Molecule: Crystallography, 3D Hydrogen-Bonded, Fluorescence… DOI: http://dx.doi.org/10.5772/intechopen.90271*

#### **Table 4.**

The absorption spectra of the studied compound are shown in **Figure 1**. The computed absorption bands, dominant transitions, characters and oscillator

respectively; and these transitions are affected to a π-π\* transition.

Bader and Essen have shown that that the negative value of ∇<sup>2</sup>

which implies the presence of a hydrogen-bonding interaction [16, 17].

point between all of each two bonded atoms in part B.

those obtained by experimental refinement.

**Table 3.**

**Figure 4.**

**82**

*TD-DFT absorption spectra of phh.*

The compound phh that absorbs in the region (λ = 165–280 nm) appears in **Figure 4**, and it shows three peaks with maxima at λ = 190, 225 and 268. **Table 3** clearly indicates that the lowest energy and the intense peak is at λ = 268 nm (E = 4.62 eV), transition character as corresponding it results from a transition H2 to L+1**.** From **Figure 4** we observe two absorption peaks positioned at λ = 225 and 190 nm; the absorption bands correspond to the H1 to L+3 and H3 to L+2,

there is an electronic charge concentration at the BCP, which implies that the nature of the bond is covalent. For intermolecular interactions, is less weak and ∇ > 0,

The atoms in molecules (AIM) theory for part B (C1B to C12B/O1W) was applied to analyze the electron densities and their properties; details obtained from this approach are shown in **Table 4**. **Figure 5** shows the existence of a bond critical

We notice from **Table 4**, the values ρ > 0.2 and Δ < 0 indicate that covalent bonds are present. And for the bond between N1B and H11W, we notice that ρ = 0.034 is very weak and Δ = 0.091 > 0 (see **Table 4**) which indicate the presence of a strong hydrogen-bonding interaction. These results are in good agreement with

**λ (nm) f E (ev) Transition Character** 0.48 4.62 H2 to L+1 π-π\* 0.47 5.49 H1 to L+3 π-π\* 0.20 6.49 H3 to L+2 π-π\*

*The calculated optical transition energies and their corresponding oscillator strengths (f) for phh.*

(ρ) indicates that

strengths (f) are given in **Table 3**.

*Electron Crystallography*

**5.2 AIM topological analysis**

*Results of atoms in molecule approach for part B of phh molecule.*

**Figure 5.** *The critical point founded between every pair of atoms in part B.*

#### **5.3 Orbital analysis and molecular electrostatic potential**

The energy diagram of the molecular orbitals obtained by DFT approach for part B of compound phh is shown in **Figure 6**.

The HOMO and LUMO are important orbitals in a molecule; the gap between the occupied and vacant orbitals (HOMO/LUMO) is remarkable in the compound (2.92 eV; see **Figure 6**) and predicts its stability.

The highest occupied molecular orbital (HOMO) is mainly delocalized on the oxygen atom (93%), while it is found that the carbons of the cycles contribute strongly in the composition of the LUMO orbital with a participation rate of 88%.

The molecular electrostatic potential is a very important element for the illustration and visualization of the charge region variability and allows identifying the electrophilic and nucleophilic attack sites as well as the hydrogen-bonding interactions [18–21].

The blue region represents positive MESP, and the red region represents negative ESP, while the green region refers to the neutral region. From the MESP surface diagram, it can be seen that negative regions (red) are mainly localized over the oxygen and the nitrogen atom, while the positive regions (blue) are distributed over *Electron Crystallography*

The crystals formed were washed and filtered using 20 ml of water.

(1): 3400 (vs), 3084 (m), 1632 (w), 1617 (w), 1575 (s), 1564 (m), 1502 (s), 1443 (w), 1414 (vs), 1340 (w), 1285 (vw), 1208 (w), 1132 (m), 1082 (w), 1031 (w), 987

*Strongly Fluorescent Heterocyclic Molecule: Crystallography, 3D Hydrogen-Bonded, Fluorescence…*

Computer programmes by Bruker *APEX2* (2006) [22]; *SAINT* (Bruker, 2006) [22]; *SAINT*, *SIR2002* [23], and *SHELXL2008* [24]; *WinGX* [25]; *Mercury* Version 1.4 [26]

Crystal data, data collection and structure refinement details are summarized in **Table 5**. H atoms were placed at calculated positions with C▬H = 0.93 Å (aromatic

Chemical formula C13.50H11.25N2.25O1.13

a, c (Å) 17.5075 (7), 8.4300 (4)

) 2237.72 (14)

) 0.09 Crystal size (mm) 0.2 0.1 0.08

Diffractometer Bruker APEX-II CCD

) 0.596

) 0.25, 0.19

Absorption correction —

Rint 0.046

Absolute structure [27] Absolute structure parameter 0.4 (15)

R[F2 > 2σ(F2)], wR(F2), S 0.047, 0.098, 1.06 No. of reflections 5115 No. of parameters 418 No. of restraints 10

Mr 223.00 Crystal system, space group Trigonal, P31 Temperature (K) 293

Z 8 Radiation type Mo Kα

):

**(hpp) Crystal data**

**Data collection**

13,243, 5115, 4195

**Refinement**

The most important infrared wavelength (cm<sup>1</sup>

(m), 860 (vw), 764 (w), 733 (vs).

*DOI: http://dx.doi.org/10.5772/intechopen.90271*

**7. Programmes**

**8. Refinement**

V (Å<sup>3</sup>

μ (mm<sup>1</sup>

No. of measured, independent and observed [I > 2σ(I)] reflections

(sin θ/λ)max (Å<sup>1</sup>

Δρmax, Δρmin (e Å<sup>3</sup>

**Table 5.**

**85**

*Experimental details.*

**Figure 6.** *Frontier molecular orbital diagram of part B.*

**Figure 7.** *MEP surface diagram of part B.*

the H atoms. **Figure 7** shows the presence of a hydrogen-bonding interaction between N1B and H11W.
